This is an open access article published under an ACS AuthorChoice License, which permits copying and redistribution of the article or any adaptations for non-commercial purposes.
Research Article http://pubs.acs.org/journal/acscii
Colloidal Covalent Organic Frameworks Brian J. Smith,†,‡ Lucas R. Parent,§ Anna C. Overholts,† Peter A. Beaucage,∥ Ryan P. Bisbey,†,⊥ Anton D. Chavez,†,⊥ Nicky Hwang,† Chiwoo Park,# Austin M. Evans,⊥ Nathan C. Gianneschi,*,§,○ and William R. Dichtel*,†,⊥ †
Department of Chemistry and Chemical Biology and ∥Department of Materials Science and Engineering, Cornell University, Ithaca, New York 14853, United States ‡ Department of Chemistry, Bucknell University, Lewisburg, Pennsylvania 17837, United States § Department of Chemistry & Biochemistry and ○Materials Science & Engineering, University of California, San Diego, La Jolla, California 92093, United States ⊥ Department of Chemistry, Northwestern University, Evanston, Illinois 60208, United States # Department of Industrial and Manufacturing Engineering, Florida State University, Tallahassee, Florida 32306, United States S Supporting Information *
ABSTRACT: Covalent organic frameworks (COFs) are twoor three-dimensional (2D or 3D) polymer networks with designed topology and chemical functionality, permanent porosity, and high surface areas. These features are potentially useful for a broad range of applications, including catalysis, optoelectronics, and energy storage devices. But current COF syntheses oﬀer poor control over the material’s morphology and ﬁnal form, generally providing insoluble and unprocessable microcrystalline powder aggregates. COF polymerizations are often performed under conditions in which the monomers are only partially soluble in the reaction solvent, and this heterogeneity has hindered understanding of their polymerization or crystallization processes. Here we report homogeneous polymerization conditions for boronate ester-linked, 2D COFs that inhibit crystallite precipitation, resulting in stable colloidal suspensions of 2D COF nanoparticles. The hexagonal, layered structures of the colloids are conﬁrmed by small-angle and wide-angle X-ray scattering, and kinetic characterization provides insight into the growth process. The colloid size is modulated by solvent conditions, and the technique is demonstrated for four 2D boronate ester-linked COFs. The diameter of individual COF nanoparticles in solution is monitored and quantiﬁed during COF growth and stabilization at elevated temperature using in situ variable-temperature liquid cell transmission electron microscopy imaging, a new characterization technique that complements conventional bulk scattering techniques. Solution casting of the colloids yields a free-standing transparent COF ﬁlm with retained crystallinity and porosity, as well as preferential crystallite orientation. Collectively this structural control provides new opportunities for understanding COF formation and designing morphologies for device applications.
INTRODUCTION Covalent organic frameworks (COFs) are crystalline porous polymers with predictable bonding in two or three dimensions, tunable molecular structures, and high speciﬁc surface areas.1−5 COFs are potentially attractive for selective membranes, catalyst supports, organic electronic devices, and electrical energy storage devices.6−15 One of the major challenges to harnessing their properties is that COFs are typically formed as insoluble microcrystalline powders, which are diﬃcult to process or not useful for these applications. Although some progress has been made in preparing COF thin ﬁlms selectively and with speciﬁc crystalline orientations,16−18 we attribute the small average crystallite sizes and tendency to form as powders to empirical screening approaches used to identify polymerization conditions for new frameworks. We recently reported the ﬁrst studies into the mechanism of COF growth using © 2017 American Chemical Society
boronate ester systems as a model network, which identiﬁed an irreversible precipitation during the reaction that inhibited further structural error correction and crystallite growth.19 We hypothesized that this aggregation of crystallites was a function of both rapid, facile nucleation and intermolecular attractive forces between the crystallites. Here we report a synthetic approach to arrest irreversible crystallite aggregation and precipitation, resulting in the ﬁrst stable colloidal suspensions of COF nanoparticles. The resulting colloids show characteristic COF crystallinity, with adjustable particle size, low polydispersity, and long-term stability. We demonstrate the ﬁrst use of in situ variabletemperature liquid-cell transmission electron microscopy (VTReceived: November 5, 2016 Published: January 12, 2017 58
DOI: 10.1021/acscentsci.6b00331 ACS Cent. Sci. 2017, 3, 58−65
ACS Central Science
Figure 1. (A) Typical growth conditions for boronate ester-linked 2D COFs provide insoluble, polycrystalline powders. CH3CN cosolvents instead yield stable colloidal nanoparticles of the crystalline polymer networks. (B) Colloid formation as a function of solvent CH3CN percentage (2 mM HHTP, 1.5 equiv of PBBA, 15 equiv of CH3OH, remaining solvent 4:1 dioxane/mesitylene, 90 °C).
actions between particles. Such interactions are not unexpected given that acetonitrile stabilizing agents stand in notable contrast to bulky or amphiphilic ligands often used in nanoparticle syntheses. Colloid formation is speciﬁc to nitrile cosolvents, whereas other cosolvents (e.g., CH2Cl2, THF, toluene) result in COF-5 precipitation (Figure S1B and Table S1). Benzonitrile also stabilizes colloid growth, suggesting that a direct interaction between the nitrile functional group and the COF is responsible for colloid formation. Control experiments, in which each monomer was subjected to the polymerization conditions in the absence of the other, show no evidence of nanoparticle formation, ruling out the formation of simple monomer aggregates. Taken together, these observations indicate that nitrile solvents uniquely inhibit the precipitation of COF-5 as a microcrystalline powder. These reaction conditions provide a previously unattainable means to characterize COF formation and allow for subsequent solution processing. In-Situ Small-Angle and Wide-Angle X-ray Scattering. The crystallinity and size of the COF-5 colloidal nanoparticles were characterized by small-angle and wide-angle X-ray scattering (SAXS/WAXS). Aliquots of polymerizations performed in the presence of 55% CH3CN (2 mM [HHTP]0, 90 °C) were monitored at various time points to simultaneously characterize the increase of particle size and crystallization (Figure 2). COF crystallization is observed within 15 min, as determined by the appearance of a peak at 0.24 Å−1, corresponding to the diﬀraction peak of COF-5. The integrated area of this peak increases for the initial 2 h of the polymerization, which matches the time scale of the increase in particle size calculated from the SAXS data, suggesting that the earliest observable boronate ester-linked particles are already crystalline. This behavior is consistent with our previous study of boronate ester-linked COF precipitation, in which powders isolated in the ﬁrst few minutes of the polymerization were both microcrystalline and showed high BET surface areas (>2000 m2/g).19 In contrast, 2D imine-linked COFs form an initial amorphous phase that crystallizes slowly over extended reaction times.23
LCTEM) with on-chip heating to directly image hundreds of individual COF nanoparticles as they form in solution. The colloidal COFs also allow postsynthetic solution casting to produce free-standing, porous COF ﬁlms. We anticipate this synthetic approach to both provide a fundamental understanding of COF nucleation and growth as well as facilitate device incorporation through increased morphological control of solution processable ﬁlms. Stable suspensions of porous nanoparticles also oﬀer functional internal surfaces that may prove attractive for drug delivery, chemical sensing, or siteisolated catalysts. 20,21 More broadly for the ﬁeld of solvothermal nanomaterials synthesis, these ﬁndings establish VT-LCTEM as a powerful analytical tool that complements in situ bulk scattering (light or X-ray) methods for characterizing the size, morphology, and growth processes of nanostructures in liquid.
RESULTS AND DISCUSSION Colloid Synthesis. Stable COF colloids form under conditions that disrupt crystallite aggregation yet do not inhibit polymerization. In our previous studies of 2D boronate esterlinked COF formation, the reaction temperature, monomer identity and concentration, and the addition of competitors each inﬂuence the rate of COF formation,19,22 but the resulting microcrystalline powders exhibit reasonably consistent crystalline domain sizes and morphologies. Upon evaluating various cosolvents to determine their interaction with the formation of COF-5, a prototypical 2D boronate-ester linked COF, we found that CH3CN, even at modest volume fractions, prevents precipitation and provides stable colloidal COF-5 suspensions. Speciﬁcally, the condensation of 2,3,6,7,10,11-hexahydroxytriphenylene (HHTP) and 1,4-phenylenebis(boronic acid) (PBBA) to form COF-5 under homogeneous conditions (2 mM HHTP, 3 mM PBBA, 4:1 dioxane/mesitylene, 90 °C), modiﬁed to include 15−95 vol % CH3CN, provides a translucent solution that exhibits a pronounced Tyndall eﬀect (Figures 1 and S1A). No precipitation occurs from the reaction mixture upon cooling, even after standing for weeks. However, it is possible to sediment these particles through extended centrifugation, suggesting transient and/or reversible inter59
DOI: 10.1021/acscentsci.6b00331 ACS Cent. Sci. 2017, 3, 58−65
ACS Central Science
and inhibits their aggregation. The earliest observed particle sizes are comparable to the 20−40 nm crystalline domains determined by X-ray diﬀraction of COF-5 precipitated powders previously synthesized in the absence of CH3CN.19 Concurrently, the standard deviation of the particle size distribution narrows as the particles grow. COF crystallites undergo further growth after nucleation, which slows over time, presumably due to monomer consumption. CH3CN stabilizes colloids of several boronate ester-linked COFs, indicating the generality of this procedure. HHTP was reacted with 4,4′-biphenylbis(boronic acid), 2,7-pyrenebis(boronic acid), and 4,4′diphenylbutadiynebis(boronic acid) under similar conditions to yield colloids of COF-10,24 TP-COF,25 and HHTP-DPB COF,26 respectively. The crystallinity of each COF colloidal suspension was conﬁrmed by the presence of its diﬀraction peak in the WAXS pattern (Figure 2C). The feature at 0.16 Å−1 corresponds to the of HHTP-DPB COF, in addition to the peak observed at 0.27 Å−1. The WAXS patterns for COF-10 and TP-COF are consistent with the expected structures and resolve the slight diﬀerence in the length between the biphenyl and pyrene linkages. The kinetics of DPB-HHTP COF colloid formation were similar to that of COF-5, with framework crystallinity again observed at the earliest time points at which particle size is detectable (Figure S5). These combined observations demonstrate the generality of the colloidal stabilization of 2D boronate ester-linked COFs by the CH3CN cosolvent. It is therefore likely that CH3CN interacts directly with the boronate linkages to attenuate attractive forces between crystallites. Colloid Size Characterization and Control. Dynamic light scattering (DLS) was used to probe the long-term stability of COF-5 colloidal suspensions and the eﬀect of the polymerization conditions on particle size. The average particle size and polydispersity index were measured for reaction mixtures of varying monomer and CH3CN concentrations after their polymerization at 90 °C for 20 h (Figure 3 and Table S2). For all CH3CN concentrations examined (15−95 vol % CH3CN), the colloids exhibit Gaussian size distributions and low polydispersity indices. The average particle size is relatively invariant at CH3CN concentrations above 55 vol %, between 45−60 nm. This size is comparable to the 20−40 nm crystallite sizes observed by powder X-ray diﬀraction (PXRD) of COF-5 precipitates and suggests stabilization of discrete crystallites at high CH3CN concentrations. Larger colloids (100 and 240 nm) are obtained at 15 and 35 vol % CH3CN, respectively. These larger particle sizes may originate from the aggregation of discrete, smaller crystallites at lower CH3CN content, which would represent a transition from insoluble material with no added CH3CN to dispersed, smaller colloids at higher CH3CN content (Figure 3). COF colloid growth conditions yield monodisperse particle distributions, with DLS PDI < 0.2. The initial monomer concentration has a minor inﬂuence on the particle size, with an average of 60 nm at 2 mM [HHTP]0 and 75 vol % CH3CN. This average decreases to 40 nm at 1 mM [HHTP]0 under similar reaction conditions (Figure 3B). Once formed at a given CH3CN concentration, the colloids are stable for at least one month at room temperature (Table S2). Furthermore, the particle sizes do not change if the CH3CN concentration is varied after the colloids have been formed. For example, 230 nm colloids formed at 15 vol % CH3CN do not shrink when additional CH3CN is added to the solution. Likewise, 50 nm colloids do not increase in size when diluted by non-nitrile containing cosolvents, even upon heating
Figure 2. (A) SAXS/WAXS of in situ COF-5 colloid formation over time, with inset of the highlighted diﬀraction peak (growth conditions: 2 mM HHTP, 1.5 equiv of PBBA, 15 equiv of CH3OH, solvent 55% vol % CH3CN, 90 °C). (B) Particle size and diﬀraction integrated area as a function of time. (C) WAXS diﬀraction peaks of boronate ester COF colloids prepared using various boronic acid linkers (red: COF-5; green: COF-10; blue: Py-COF; purple: HHTP-DPB COF), indicating the generality of this procedure.
The colloidal COF nanoparticles have relatively uniform size distributions, as is evident from the measurable SAXS form factor (Figures 2 and S4). Particle sizes are quantiﬁable at 25 min at a mean radius of 21 nm, which increases to 30 nm in the initial 2 h. This increased particle size is accompanied by an increase in the intensity of the reﬂection, which suggests that the particle growth occurs through polymerization and crystallization processes rather than particle aggregation. Furthermore, the particle size distribution narrows as the average crystallite size increases, characterized by the full-width half max (fwhm) of the peak, which is also inconsistent with particle aggregation (Figure S4). These observations indicate that CH3CN stabilizes discrete crystallites in solution 60
DOI: 10.1021/acscentsci.6b00331 ACS Cent. Sci. 2017, 3, 58−65
ACS Central Science
Figure 3. Average size of COF-5 colloidal nanoparticles prepared under diﬀerent reaction conditions, characterized by the DLS Z-average, where error bars correspond to the polydispersity width. (A) Size dependence as a function of the volume fraction of CH3CN (remainder is 4:1 dioxane/ mesitylene). (B) Size dependence as a function of [HHTP]0 at 75% vol % CH3CN.
at 90 °C (Figure S6). These experiments demonstrate that COF colloids are stable and robust once formed. Therefore, the particles are likely not in rapid equilibrium but rather kinetically trapped without appreciable monomer exchange. This suggests that crystallite size limitation in COF growth is not due to precipitation, but rather a lack of Oswald ripening postnucleation. Colloid stability provides the opportunity to explore a variety of postsynthetic processing to characterize and control overall morphology. To further explore the size of colloidal particles, solvated colloidal nanoparticles were dried and analyzed by atomic force microscopy (AFM). COF-5 colloids are readily drop cast onto mica, yielding discrete surface-adsorbed species (Figure 4). COF nanoparticles size trends are consistent with DLS measurements, with smaller particles observed at CH3CN solvent levels >55%. In particular, average heights at 95% CH3CN are